www.rsc.org/chemcomm | ChemComm
High contrast solid state electrochromic devices based on Ruthenium Purple nanocomposites fabricated by layer-by-layer assemblyw Vaibhav Jain,a Rabindra Sahoo,b Joerg R. Jinschek,c Reza Montazami,d Hank M. Yochum,e Fredrick L. Beyer,f Anil Kumarb and James R. Heﬂin*d Received (in Cambridge, UK) 6th March 2008, Accepted 6th May 2008 First published as an Advance Article on the web 12th June 2008 DOI: 10.1039/b803915a
Electrochromic Ruthenium Purple–polymer nanocomposite ﬁlms, fabricated by multilayer assembly, were found to exhibit sub-second switching speed and the highest electrochromic contrast reported to date for any inorganic material. In the last two decades, the only inorganic non-oxide materials that have attracted signiﬁcant attention for incorporation in low power electrochromic displays are those belonging to the metal hexacyanoferrate (HCNF) family.1 In the HCNF family, Prussian Blue (PB) is by far the most studied electrochromic material. In contrast, Ruthenium Purple (RuP) has not been explored for electrochromic displays because the neutral form is insoluble in aqueous solution. Though nanocomposites incorporating polymer and inorganic materials have shown improved performance as compared to the separate constituents in terms of mechanical stability, electrochemical activity, and solar energy conversion,2 their use in electrochromic devices has not been well studied. In this paper, we describe the synthesis of stable Ruthenium Purple nanoparticles and the electrochromic and surface properties of Ruthenium Purple–polymer nanocomposites fabricated by the layer-by-layer (LbL) assembly approach. RuP belongs to the class of well-deﬁned zeolite-like polynuclear inorganic materials with ﬁxed metal ionic redox centers (e.g., Ru(II) and Fe(III)) wherein the electroneutrality is maintained during the redox process by the movement of freely diﬀusing cations in and out of the lattice structure.3 As discussed by several groups and similar to PB, RuP is present in two forms: ionized water-soluble KFeIII[RuII(CN)6]xH2O and a neutral insoluble compound, FeIII4[RuII(CN)6]3.4–7 The soluble RuP is present in a colloidal form and the inclusion of potassium makes it stable in aqueous media, bringing an overall negative charge, which allows LbL assembly using RuP colloids as the anions. As explained by Rosseinsky et al.,8 the incorporation of K+ as a ‘supernumerary’ cation in FeIII[RuII(CN)6] makes it water-soluble. RuP (FeIII4[RuII(CN)6]3/KFeIII[RuII(CN)6]xH2O) in its natural form has a deep purple color and
changes to colorless Ruthenium White (RW), FeII3[RuII(CN)6]2 upon reduction. For the present studies, synthesis of 5 mM solution of RuP was carried out by mixing equal concentrations of potassium ruthenium cyanide (K4[Ru(CN)6]), ferric chloride (FeCl3) and potassium chloride (KCl). KCl is added to ensure the excess of potassium ions crucial for the solubility of RuP. This was further puriﬁed by ultraﬁltration to remove insoluble RuP, following the procedure described by DeLongchamp et al.7 The composition of the as-synthesized product in powder form was conﬁrmed by the X-ray diﬀraction (XRD) pattern (Fig. 1). The main peaks at 16.91 (200), 23.81 (220), 34.11 (400), 38.21 (420), and 44.31 (420) can be readily indexed as a pure face-centered cubic (fcc) phase of RuP [space group: Fm3m]. The broadening of the XRD is known to occur when the particle size reduces progressively below 200 nm.9 The values are in good agreement with values reported by other groups for RuP and its analogs.6,10,11 Transmission electron microscopy (TEM) (Fig. 2) and dynamic light scattering (DLS) (see ESI Fig. S2(a)w) of the sample were taken from the diluted RuP solution and both techniques show that the average RuP nanoparticle size is 20–30 nm, which is in the range of values reported for HCNF nanoparticles by other groups.7,12 RuP possesses a simple fcc lattice structure;13,14 the metal ion centers in the fcc structure are Ru(II) and Fe(III) with cyanide groups between these ions. The presence of (200) fcc structure is conﬁrmed by a fast
Macromolecular Science and Engineering, Virginia Tech, Blacksburg, USA Department of Chemistry, IIT-Mumbai, Mumbai, India c Materials Science and Engineering, Virginia Tech, Blacksburg, USA d Department of Physics, Virginia Tech, Blacksburg, USA. E-mail: rheﬂ[email protected]
e Department of Physics and Engineering, Sweet Briar College, USA f Materials Division, Army Research Laboratory, Aberdeen, USA w Electronic supplementary information (ESI) available: Experimental details. See DOI: 10.1039/b803915a b
This journal is
The Royal Society of Chemistry 2008
Fig. 1 An XRD pattern of the powder form of the RuP sample, conﬁrming the formation of pure fcc Fe4[Ru(CN)6]3. The inset is the unit cell of Fe4[Ru(CN)6]3.
Chem. Commun., 2008, 3663–3665 | 3663
Fig. 2 TEM image (a) of the nanoparticles and FFT diﬀraction pattern (inset) of one of the marked nanoparticles; (b) shows the d-spacing values.
Fourier transform (FFT) image (inset of Fig. 2(a)) of the TEM diﬀraction pattern and is in agreement with the XRD results. The d-spacing value of 2.3 A˚ measured by TEM (Fig. 2(b)) for a crystal lattice (420) within the RuP nanoparticles with a lattice constant, a = 10.26 A˚ is in good agreement with the standard values for bulk cubic RuP.15 Zeta potential measurements (see ESI Fig. S2(b)w) also conﬁrmed the presence of two kinds of hexacyanoferrates, one of higher content (490%) with a negative potential value of 30.0 mV and the other low content insoluble part (o10%) of value 2.5 mV. The amount of negative charge carried by soluble RuP nanoparticles is suﬃcient to fabricate ﬁlms by LbL assembly. Though the colloidal dispersion of RuP nanoparticles is stable for months, sonication for 15–20 min before deposition results in better ﬁlms due to breaking of the agglomerates. Although the LbL approach has been used in the formation of (all-inorganic) PB and RuP multilayers on electrode surfaces,6 the application of this technique in the production of hybrid polymer–inorganic nanocomposite ﬁlms has so far been reported only for PB combined with either linear polyethylene imine (LPEI)7 or polyaniline (PANI)16 as the polymeric materials, but none has been reported for RuP. Herein, we show for the ﬁrst time an adaptation of this approach to the formation of LPEI–RuP nanocomposite multilayered ﬁlms with improved electrochromic properties. The LbL assembly approach introduced by Decher et al.17 provides nanoscale control of multilayer ﬁlm thickness. For LbL assembly, indium tin oxide (ITO) coated glass substrates were alternately immersed in 10 mM solution of LPEI at pH 4 and 5 mM solution of RuP at pH 4. Further details are provided in ESI.w X-Ray photoelectron spectroscopy data (see ESI Fig. S3w) of the 40-bilayer LbL ﬁlm (with an outermost layer of the ﬁlm of RuP nanoparticles) of LPEI–RuP further showed almost 1 : 1 atomic concentration of Ru and Fe, conﬁrming the presence of soluble RuP nanoparticles in the ﬁlms, while higher ratios of Ru to Fe would have indicated the presence of extra Ru(II) occupying interstitial K+ cationic sites in [RuII(CN)6]4 lattice vacancies and making it insoluble. Spectroelectrochemistry studies of the RuP nanocomposite ﬁlms in solution show the color change from purple–violet color to transparent as a negative voltage is applied. The absorption spectra from +1 V to 1 V, in 0.1 V steps, of a 40-bilayer ﬁlm of LPEI–RuP nanocomposite are presented in Fig. 3. An exceptionally large change in transmittance of greater 3664 | Chem. Commun., 2008, 3663–3665
Fig. 3 Spectroelectrochemistry data of the absorbance of a 40-bilayer RuP ﬁlm in 0.1 M LiClO4–ACN solution on increase of voltage from +1 V to 1 V in 0.1 V steps.
than 84% at a wavelength of 560 nm is observed as the ﬁlm becomes transparent (RW) from the purple–magenta color (RuP). This is, to our knowledge, the highest contrast reported to date for any inorganic electrochromic material. The contrast values reported by DeLongchamp et al. are 77% (60 bilayers) and 61% (30 bilayers) for LPEI–PB7 and PANI–PB,16 respectively. There is no report of coloration eﬃciency or solid-state switching measurements in those publications. Cyclic voltammetry (CV) was performed on the LPEI–RuP nanocomposite between 0.5 V to 1.0 V, which is the potential range expected for the RuP to RW transition (see ESI Fig. S4w). LPEI is an inactive polyelectrolyte, so the RuP controls the electrochemistry of the nanocomposite as conﬁrmed by the agreement with the redox potential values of RuP found by other groups.18 The reduction peak for RuP to RW was observed at 0.05 V which is in agreement with the reported values.5,7 The corresponding oxidation peak was observed at 0.23 V in the reverse scan. The electrochemical reaction for the 40-bilayer LPEI–RuP nanocomposite ﬁlm is completely reversible at low scan rates up to 50 mV s 1, which shows that even thick ﬁlms (41 mm) are fully electrochemically accessible. At higher scan rates the ﬁlm is partially reduced and the sharp peaks of oxidation and reduction broaden and become ﬂat. The broadening of the peaks is attributed to the presence of inactive LPEI present in the nanocomposite ﬁlm; this increases the internal resistance of the ﬁlm and the Li+ ion insertion from the electrolyte to the electrochemical sites is more diﬃcult. As explained by Ellis et al.,19 at low scan rates the shape of the cyclic voltammogram is controlled more by the thermodynamic than the kinetic factors. The overall reaction mechanism does not change for diﬀerent electrolytes but as reported by Chen et al.,20 the E1 values of the RuP seem to be aﬀected by the type of cation (H+, Li+, Na+, K+, Rb+) in the electrolytic solutions. This could be due to the size of the cation, which plays an important role in the electrochemical behavior of the RuP ﬁlms due to its inclusion and expulsion in the crystal lattice during potential cycling. According to the above discussion, This journal is
The Royal Society of Chemistry 2008
Fig. 4 Solid-state switching of a device (measured at 633 nm) consisting of a 40-bilayer LPEI–RuP ﬁlm as a cathodically coloring material and a 40-bilayer PANI–PAMPS ﬁlm as the anodically coloring material at 1 V to +0.8 V.
the redox reaction of the RuP in the case of Li+ cations can be written as: KFeIII[RuII(CN)6] + Li+ + e 2 LiKFeII[RuII(CN)6] (1) 2
The coloration eﬃciency was found to be 205 cm C for the present LPEI–RuP nanocomposites and is one of the highest reported for any inorganic electrochromic material. The charge per unit area required for the reduction process of RuP to RW is 4.16 mC cm 2 for a 40-bilayer ﬁlm, which is the same number of bilayers used for CV, optical switching and UV–Vis absorption data. The Faradic charge associated with one bilayer for the process is 105 mC cm 2 and the surface coverage for each bilayer can be calculated by G = Q/nF where F is the Faraday constant (96.5 103 sA mol 1). The surface coverage calculated using the above equation was found to be 1.1 10 9 mol cm 2. This agrees well with the surface coverage expected for RuP nanoparticles of this size.21 Optical switching of RuP nanocomposite ﬁlms was performed in both liquid electrolyte (see ESI Fig. S5w) and in solid-state devices. Solid-state devices were fabricated by depositing the LbL ﬁlm on ITO coated glass in the same way as described in our previous work.22 Two separate 40bilayer ﬁlms of PANI–poly(2-acrylamido-2-methylpropanesulfonic acid) (PAMPS) and LPEI–RuP were taken as complementary anodically and cathodically coloring materials, respectively. The LiClO4–PC gel polyelectrolyte used for the solid-state device was synthesized as described by Sonmez et al.23 The solid-state device switches from light blue to dark purple with coloration and decoloration times in the range of 600 ms and 300 ms, respectively, as shown in Fig. 4. The switching speed can potentially be improved by replacing LPEI with a cationic conducting polymer such as PANI, poly(phenylene vinylene) (PPV) etc. This is one of the ﬁrst This journal is
The Royal Society of Chemistry 2008
nanocomposite solid-state electrochromic devices reported in the literature. In conclusion, RuP nanoparticles with spherical morphology were synthesized and thin ﬁlm polymer–RuP nanocomposites were fabricated by the LbL technique. The absorbance of the ﬁlm increases linearly with the number of bilayers deposited, indicating that thick nanocomposite ﬁlms can be easily fabricated without sacriﬁcing the individual contributions of the constituents. The 40-bilayer nanocomposite ﬁlms show a very high contrast of around 84% with a high coloration eﬃciency of 205 cm2 C 1. The change in color from purple–red (magenta) to transparent and switching in solidstate devices also ﬁlls in the gap in tri-color space of cyan, magenta, yellow (CMY) reﬂective displays described by DeLongchamp et al.7 In this communication, our aim is to show the synthesis of RuP nanoparticles and the electrochromic properties of the polymer–RuP nanocomposites. Detailed electrochemical and multi-chromic studies and the eﬀect of other polyelectrolytes will be presented in our forthcoming papers. This material is based upon work supported in part by the U.S. Army Research Oﬃce under grant number W911NF-071-0452 Ionic Liquids in Electro-Active Devices (ILEAD) MURI.
Notes and references 1 C. G. Granqvist, Handbook of Inorganic Electrochromic Materials, Elsevier, Amsterdam, 1995. 2 K. Rajeshwar, N. De Tacconi and C. R. Chentahmaramakrishnan, Chem. Mater., 2001, 13, 2765. 3 I. Carpani, M. Giorgetti, M. Berrettoni, P. L. Buldini, M. Gazzano and D. Tonelli, J. Solid State Chem., 2006, 179, 3981. 4 K. Itaya, I. Uchida and U. D. Neﬀ, Acc. Chem. Res., 1986, 19, 162. 5 A. Jaiswal, J. Collins, B. Agricole, P. Delhaes and S. Ravaine, J. Colloid Interface Sci., 2003, 261, 330. 6 R. C. Milward, C. E. Madden, I. Sutherland, R. J. Mortimer, S. Flecher and F. Marken, Chem. Commun., 2001, 1994. 7 D. M. DeLongchamp and P. T. Hammond, Adv. Funct. Mater., 2004, 14, 224. 8 D. R. Rosseinsky and A. Glide, J. Electrochem. Soc., 2003, 150(9), C641. 9 A. R. West, Solid State Chemistry and its applications, John Wiley and Sons, Chichester, 1990, p. 173. 10 M. Cao, X. Wu, X. He and C. Hu, Chem. Commun., 2005, 2241. 11 Y. Song, W. Jia, Y. Li, X. Xia, Q. Wang, J. Zhao and Y. Yan, Adv. Funct. Mater., 2007, 17, 2808. 12 N. Bagkar, R. Ganguly, S. Choudhury, P. A. Hassan, S. Sawant and J. V. Yakhmi, J. Mater. Chem., 2004, 14, 1430. 13 H. Inoue and S. Yanagisawa, J. Inorg. Nucl. Chem., 1974, 36, 1411. 14 M. V. Bennett, L. G. Beauvais, M. P. Shores and J. R. Long, J. Am. Chem. Soc., 2001, 123, 8022. 15 A. Ludi and H. U. Gudel, in Structure and Bonding, ed. J. D. Dunitz, Springer Verlag, New York, 1973, ch. 1, vol. 14, p. 8. 16 D. M. DeLongchamp and P. T. Hammond, Chem. Mater., 2004, 16, 4799. 17 G. Decher, Science, 1997, 227, 1232. 18 K. Sone and M. Yagi, Macromol. Symp., 2006, 235, 179. 19 D. Ellis, M. Eckhoﬀ and V. D. Neﬀ, J. Phys. Chem., 1981, 85, 1221. 20 S. Chen and S. Hsueh, J. Electroanal. Chem., 2004, 566, 291. 21 S. Liu, D. G. Kurth, H. Mohwald and D. Volkmer, Adv. Mater., 2002, 14, 225. 22 V. Jain, H. M. Yochum, H. Wang, R. Montazami, M. A. V. Hurtado, A. Mendoza-Galva´n, H. W. Gibson and J. R. Heﬂin, Macromol. Chem. Phys., 2008, 209, 150. 23 G. Sonmez, H. Meng and F. Wudl, Chem. Mater., 2004, 16, 574.
Chem. Commun., 2008, 3663–3665 | 3665